Measurement of antibacterial properties
of foil‑backed electrospun nanofibers
Mary Ann Wagner‑Graham1*
, Herbert Barndt2
and Mark Andrew Sunderland3
The use of electrospinning to create novel nanoscale materials is increasing, along with potential biomedical applications for nanofibers made from natural, sustainable materi-als (Bhardwaj and Kundu 2010). In this process, nanofibers are deposited on a metallic foil support, and held in place by electrostatic interactions. Since the resulting material is poorly absorbent, and the nanofibers are easily disturbed and lifted from the foil back-ing, assessment of their antibacterial properties through use of existing methods is not possible.
The American Association of Textile Chemists and Colorists (AATCC) recom-mends the AATCC 100 protocol to assess antibacterial properties of fabrics. However, this protocol requires complete absorbance of a standard volume of bacterial inocu-lum by multiple swatches of absorbent fabric, and cannot be applied to poorly absor-bent swatches of aluminum foil-backed electrospun nanofibers. The Japanese Industrial Standard (JIS) Z 2801 test assesses antimicrobial properties of nonabsorbent surfaces, but nanofibers would lift from the foil backing during the testing process and carry over to the agar plates used for enumeration of remaining bacterial load, skewing the results.
Current methodologies for evaluation of antibacterial properties of traditional textiles are not applicable to foil‑backed, poorly‑absorbent electrospun nanofiber materials, since existing test methods require absorbent fabrics. Since electrospun nanofibers are adhered to the foil backing only by electrostatic interactions, methods used to evalu‑ ate antibacterial properties of surfaces cannot be used because these protocols cause the nanofibers to lift from the foil backing. Therefore, a novel method for measurement of the antibacterial properties of electrospun metallic foil‑backed nanofiber materials was developed. This method indicated that acetate‑based nanofibers manufactured to contain 5 to 30 weight percent of cold‑pressed hemp seed oil or full‑spectrum hemp extract inhibited the growth of Staphylococcus aureus in a dose‑dependent man‑ ner, from 85.3% (SEM = 2.2) inhibition to 99.3% (SEM = 0.15) inhibition, respectively. This testing method represents an advanced manufacturing prototype procedure for assessment of antibacterial properties of novel electrospun, metallic foil‑backed nanofiber materials.
Keywords: Antibacterial, Antimicrobial textiles, Nanofiber, Electrospinning, Hemp, Staphylococcus aureus
© The Author(s) 2019. This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creat iveco mmons .org/licen ses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
1 Assistant Professor
of Biology, Department of Biological and Chemical Sciences, College of Life Sciences, Thomas Jefferson University, 4201 Henry Avenue, Philadelphia, PA 19144, USA
Additionally, an investigational amount of the electrospun material may not be gener-ated in great enough quantity to provide sufficient surface area for replicate JIS Z 2801 testing.
We developed a novel testing protocol to assess the antibacterial effectiveness of ace-tate-based, aluminum foil-backed electrospun nanofibers containing different amounts of hemp oils extracted from different parts of the plant. This method requires only a small amount (two 2.5 cm2 disks) of foil-backed fibers for each replicate, permitting
multiple replicates to be run with limited material. This method may be useful to assess the antibacterial properties of other non-absorbent nanofiber materials created in small amounts using electrospinning technology.
Tryptic soy broth, tryptic soy agar, Bacto peptone, Bacto tryptone, and granulated agar were manufactured by Difco. Sodium chloride, dibasic potassium phosphate, and glu-cose were purchased from Fisher Scientific or Sigma-Aldrich. Tryptic soy agar (TSA) plates (100 mm diameter) were purchased from Teknova or prepared using TSA pow-der according to manufacturer’s directions. Methicillin-sensitive Staphylococcus aureus
subsp. aureus Rosenbach (MSSA) was purchased through American Type Culture Col-lection (ATCC #6538). Cold-pressed hemp seed oil and full-spectrum hemp extract were purchased through commercial vendors.
Preparation of the bacterial load
Staphylococcus aureus bacteria maintained in a glycerol stock were streaked for isola-tion on a TSA plate each month. Bacterial cultures (3 mL of tryptic soy broth (TSB) in sterile 13 × 100 mm borosilicate glass tubes with slip caps) were inoculated using a sin-gle colony of S. aureus grown on TSA, and incubated overnight at 37 °C with shaking at 175 rpm. The optical density (OD) 600 nm of the overnight culture was recorded using a Spectronic 20 Genesys spectrophotometer zeroed to air. When the culture in TSB was between 1.123 and 1.257 OD 600 nm, 60 to 90 µL of culture was added to a fresh 3 mL culture of TSB (initial OD 600 nm 0.051 to 0.075) for a final OD 600 nm of 0.097 to 0.109. Equal volumes (500 µL each) of this culture and TSA slurry were combined and vortexed before application to the samples.
Preparation and UV‑sterilization of the foil‑backed electrospun nanofibers
Aluminum foil-backed nanofibers were prepared using an NEU Nanofiber Electrospin-ning Unit manufactured by Kato Tech. The standard spinElectrospin-ning parameters were: target speed, 1.25 m/min; sample area, 0.1 m2; pump speed 1.5 mL/h; voltage, 18 kV. One
and a circular plastic template. Figure 1 outlines the process for UV-sterilization of the nanofiber material, along with application of the initial bacterial load. Disks were placed foil-side-up in sterile 100 mm diameter plastic culture dishes (lids removed) in a biosafety cabinet and dosed with UV light for 30 min. Then the pieces were flipped with sterile forceps, and the nanofiber-sides of the disks were treated with UV light for 30 min. Disks were repositioned on the dish so the entire inner surface of the dish was treated with UV light. Paired samples were run for each antibacterial testing trial: nanofibers containing acetate alone or nanofibers containing acetate and a percent-age of either full-spectrum hemp extract or cold-pressed hemp oil. Foil disks without nanofibers were included in some trials, and run in parallel with samples of foil-backed 100% acetate nanofibers and with acetate nanofibers incorporating 30% by weight full-spectrum hemp extract, to assess plain foil for any antibacterial effects. Figure 2 shows a schematic overview of the testing process.
Application of bacteria to the nanofiber samples
Staphylococcus aureus culture in TSA slurry (Tryptone, 17 g; Peptone, 3 g; NaCl, 8.5 g; K2HPO4, 2.5 g; glucose, 2.5 g; granulated agar, 3 g; in 1 L; autoclave 25 min, 121 °C, 15
psi) was applied to the center of the nanofiber surface of one disk, and the second disk was placed on top, nanofiber surface down. This formed a sandwich with the bacterial culture (10 µL) contained between the nanofiber surfaces, and the foil surfaces on the top and bottom of the sandwich. A sterile disposable plastic cell spreader was used to gently smooth over the top foil surface of the sandwich, ensuring good contact between the bacterial culture and the nanofiber surfaces. If any liquid culture escaped from between the two disks, the sample was discarded. Dishes were closed and samples were placed in a 1 gallon partially-closed plastic zip-lock bag with damp paper towels to pre-vent dehydration of the samples. Samples were incubated at 37 °C for exactly 4 h.
Enumeration of initial load of bacteria
The initial load of bacteria was determined by serially diluting the TSA slurry culture immediately after application of bacteria to the samples. Two independent dilution series were prepared, each beginning with 100 µL of the TSA slurry culture. Dilutions (101, 102, 103, 104, 105) were prepared by passaging 100 µL into 1.5 mL snap cap tubes
containing 900 µL sterile water. A 100 µL aliquot of the 103, 104, and 105 dilutions from
each series was applied to TSA plates, and evenly spread using a sterile disposable plastic cell spreader. Plates were inverted, and incubated overnight (18–20 h) at 37 °C.
Enumeration of bacteria recovered from foil‑backed samples
After 4 h of incubation at 37 °C, foil disks were removed from the Petri dishes, added to 10 mL of sterile water in 50 mL sterile disposable conical tubes, and vortexed for 1 min at 1200 rpm. This step recovered bacteria applied to the sample, and diluted the recov-ered bacteria by a factor of 103. Two independent serial dilutions (104, 105, 106) were
created by passaging 100 µL of the recovered bacteria through 900 µL of sterile water. For samples of foil alone, or foil with acetate alone, 100 µL from each of the 104, 105, and
106 dilutions were applied to TSA plates. For samples containing full-spectrum hemp
extract or cold-pressed hemp oil, 100 µL of the 103, 104, and 105 dilutions were plated
on TSA. Plates were incubated overnight (18–20 h) at 37 °C. Images of the plates were captured using a digital camera and colonies were counted using the Colony Counter Plugin, authored by Bruno Vieira, for ImageJ v. 1.51 k (Schneider et al. 2012).
Results and discussion
A variety of methods are available for testing antibacterial properties of traditional tex-tiles, but electrospun nanofibers are a relatively new type of material, to which exist-ing methods for assessment of antimicrobial activities of traditional absorbent fabrics or non-absorbent surfaces are not easily applied. For a tabular overview of popular existing
methods, along with a discussion of their limitations and opportunities, see the review by Teufel and Redl (2006). Unfortunately, none of the methods outlined therein are well-suited to foil-backed nanofiber materials. Multiple factors must be considered when choosing a test method, including the chemical and physical stability of the textile mate-rial and antimicrobial agent, the type of microorganism applied or recovered from the fabric, and the ultimate use of the textile. Use of a standardized testing method facilitates comparison of antimicrobial effectiveness across textile types, since different measures of antimicrobial efficacy are obtained for the same antimicrobial textile when different testing methods are applied (Haase et al. 2017). Unfortunately, a single test method can-not be applied to all textiles, as these encompass a great variety of physical and chemical properties.
The method presented here was robust and yielded reproducible results for evaluation of antimicrobial activity of electrospun nanofibers, despite application of bacterial load in a small volume (10 µL) and multiple serial dilutions performed by different techni-cians and on different days (Table 1). A 10 µL inoculum has been used in other studies focusing on long-term survival of microorganisms on fabrics (Neely and Maley 2000; Koca et al. 2012). Application of a concentrated bacterial load mimics the high bacte-rial load in exudate associated with infected skin wounds, which can exceed 108 CFU/
mL (Tachi et al. 2004). The initial bacterial loads applied to the materials in this study ranged from 4.9 × 106 to 2.0 × 108 CFU/mL, which are reasonable for use in evaluation
of a material to be used as a dressing for infected wounds.
Table 1 Reproducibility of the test method
The test procedure yielded reproducible data on different days and across different technicians
a The values shown are the percent decrease in viable bacteria recovered from the cold‑pressed hemp seed oil or full‑
spectrum hemp extract samples, as compared to the viable bacteria recovered from the paired acetate‑only samples run on the same day. All samples were on aluminum foil backing of the same type and thickness
Antimicrobial agent Technician(s) Run date % decrease of viable bacteriaa
30% full‑spectrum extract A 06/14/2017 99.5
A/B 06/19/2017 99.3
B 06/22/2017 99.0
10% full‑spectrum extract A/C 06/08/2018 97.1
A/C 06/14/2018 97.4
C 06/20/2018 97.2
C 07/02/2018 97.2
10% cold‑pressed seed oil (thin fibers) B/D 11/04/2017 90.1
A 10/02/2018 90.7
A 10/02/2018 91.2
10% cold‑pressed seed oil A/B/D 09/15/2017 91.4
B/D 09/29/2017 84.1
B/D 10/07/2017 90.1
A 10/02/2018 91.2
5% cold‑pressed seed oil C 06/28/2018 89.6
C 06/28/2018 82.3
Since the nanofibers were electrostatically associated with the aluminum foil backing, some of the nanofiber material lifted from the foil during the vortex step used to recover the applied bacteria. A control experiment was performed to determine if the antimicro-bial activity was due to carryover of plant oil from the samples to the enumeration plates. Two uninoculated UV-sterilized foil disks containing 30% or 10% full-spectrum hemp extract were added to 10 mL of sterile water and vortexed the same way as in recovery of viable bacteria. Either this solution (100 µL) or sterile water (100 µL) was applied to the surface of a sterile TSA plate and allowed to be fully absorbed into the agar before appli-cation of 100 µL of 4.8 × 107 CFU/mL bacterial inoculum. Similar amounts of bacteria,
less than two percent difference in the means, were recovered from both experimental and control plates (Table 2), indicating that observed antibacterial effects were not due to carry over of nanofiber material.
Development of this antibacterial testing method was driven by the desire to exam-ine whether plant oils or extracts provided antibacterial qualities to foil-backed ace-tate-based electrospun nanofibers. Therefore, antibacterial efficacy of the foil-backed acetate-based electrospun nanofibers made with full-spectrum hemp extract or cold-pressed hemp seed oil was quantitated as the percent reduction of viable bacteria recov-ered from those samples after a 4 h incubation at 37 °C, using the amount of viable bacteria recovered from foil-backed 100% acetate nanofiber samples, run at the same time, as a baseline. Figure 3 shows representative images of S. aureus bacterial colonies growing on TSA plates. The same load of bacteria was applied to all samples. The num-ber of bacterial colonies on the TSA plates reflect the load of viable bacteria initially applied to the samples, and the load of viable bacteria recovered from the samples after a 4 h incubation at 37 °C.
Aluminum foil can prevent bacterial growth by exclusion of atmosphere, nutrients, and moisture (Dogan et al. 2009). On the other hand, these items would be in rich sup-ply on the surface of the skin, and so aluminum foil would not be able to effect suppres-sion of bacterial growth through this mechanism if the foil-backed nanofiber material were applied in contact with skin. To determine whether aluminum foil alone, or foil-backed 100% acetate nanofibers alone, provided any antibacterial effects, initial anti-bacterial testing runs included samples of aluminum foil backing without nanofibers, in addition to foil-backed 100% acetate nanofibers and foil-backed acetate nanofibers made with cold-pressed hemp seed oil or full-spectrum hemp extract. No effective antibac-terial qualities were observed for either the aluminum foil backing without nanofibers or for foil-backed 100% acetate nanofibers alone (Figs. 3b, c, 4). Compared to the ini-tial bacterial load applied, aluminum foil backing without nanofibers permitted a 1153%
Table 2 Bacterial load of S. aureus recovered from experimental or control TSA plates
Values reported are average and standard error of the mean of bacterial load recovered
Antibacterial agent Sample Recovered bacterial load (CFU/mL)
30% full‑spectrum hemp extract Experimental 3.6 × 107± 8.0 × 105
Sterile water control 3.5 × 107± 1.2 × 106
10% full‑spectrum hemp extract Experimental 4.3 × 107± 1.5 × 106
(SEM = 278; n = 3) increase in viable bacteria after a 4 h incubation at 37 °C, while the foil-backed 100% acetate nanofibers alone allowed a 446% (SEM = 61; n = 3) increase in viable bacteria. For comparison, foil-backed acetate nanofibers containing 30% full-spectrum hemp extract by weight, run in parallel with the aluminum foil backing alone and foil-backed 100% acetate nanofiber samples, permitted only a 3% (SEM = 1; n = 3) increase in viable bacteria.
Percent reduction of viable bacteria recovered from samples made with full-spec-trum hemp extract or cold-pressed hemp oil, as compared to the acetate-only sam-ples, differed according to the concentration and source of extract or oil incorporated into the acetate-based nanofibers (Fig. 5). As expected, greater concentrations of either
Fig. 4 Foil backing without nanofibers and foil‑backed 100% acetate nanofibers lacked effective antibacterial properties. On three different days (Table 1), samples of plain aluminum foil, aluminum foil‑backed 100% acetate nanofibers, and aluminum foil‑backed acetate nanofibers containing 30% (by weight) full‑spectrum hemp extract were run in parallel. Viable S. aureus were recovered from each sample after a 4 h incubation at 37 °C. The percent increase of viable bacteria, as compared to initial load applied, is displayed. Error bars show standard error of the mean
full-spectrum hemp extract or cold-pressed hemp seed oil showed greater antibacte-rial activity. Full-spectrum hemp extract provided the greatest antimicrobial activity, as compared to cold-pressed hemp seed oil. This result agrees with literature reports on the antibacterial properties of plant-derived oils. A review by Chouhan et al. (2017) summa-rizes evidence from multiple studies showing antimicrobial activity of various plant oils differs according to the part of the plant from which they are derived. In the case of oils derived from Cannabis sativa, Lelario et al. (2018) found a greater antimicrobial activ-ity against Bacillus spp. when using oil extracted from flowers of hemp plants, as com-pared to purified cannabidiol (CBD), Δ9-tetrahydrocannabinol (THC), or a combination
of pure CBD and THC. The bioactive components of C. sativa were found in greater concentrations in flowers, as compared to seeds (Latta and Eaton 1975). The antibacte-rial properties of C. sativa are attributed to cannabinoids such as CBD (Appendino et al. 2008), which is present in low quantities in seed oil as compared to the rest of the plant (Leizer et al. 2000).
Acetate nanofibers prepared with 10% cold-pressed seed oil, stored in the dark at room temperature, showed no loss of antibacterial activity over 1 year’s time (Table 1). Thus, preliminary stability, important for practical application, has been demonstrated.
Interestingly, the 10% cold-pressed hemp seed oil material electrospun using a slower solution feed rate had a slightly higher antibacterial activity, as compared to the 10% cold-pressed seed oil material produced with the standard flow rate. A possible explana-tion for this slightly increased antibacterial efficacy is that the slower feed rate yielded thinner diameter fibers on the foil backing. The smaller diameter fibers permitted a greater ratio of nanofiber surface area per material surface area, increasing the total sur-face available for interaction with bacterial cells. A more in-depth study which varies fiber diameter would be of interest to explore this concept and determine optimal fiber diameter, since material made with a slower feed rate uses less material and is economi-cally advantageous.
The method proposed herein was designed to be used on foil-backed nanofibers, and is not appropriate to assess antibacterial properties of traditional woven or knit fabrics. There is great risk the small volume (10 µL) bacterial inoculum would not be sufficient to provide proper interaction with a large enough surface area of the threads or yarns of a woven or knit fabric, and could easily be lost through space between the yarns or threads. Lack of contact between the bacterial inoculum and the fibers of the fabric would lead to an underestimation of the antibacterial properties of the fabric. Addition-ally, reproducibility of the method from run to run would be poor.
quantitated, and the OD600 nm values reported here are valid only for S. aureus ATCC
6538 in TSB media. These numbers cannot be used for different bacteria and/or differ-ent liquid medias.
Current methods for evaluation of antimicrobial activity of textiles are difficult to apply to electrospun nanofibers. The method described herein utilized only small amounts of electrospun material, and yielded reproducible results across multiple technicians and over different days. Electrospun acetate nanofibers incorporating full-spectrum hemp extracts or cold-pressed hemp seed oils possess antibacterial properties against Staphy-lococcus aureus, and may be useful in manufacture of novel textiles with a broad range of applications in industries where control of microbial growth is desirable.
AATCC : American Association of Textile Chemists and Colorists; JIS: Japanese Industrial Standard; CBD: cannabidiol; SEM: standard error of the mean; THC: Δ9‑tetrahydrocannabinol; TSA: tryptic soy agar; TSB: tryptic soy broth.
The authors thank Claudia Papola, Deborah Wang, and Joshua Rauch of Thomas Jefferson University for their excellent technical assistance.
MAS conceptually designed hemp‑containing nanofiber material for antibacterial applications; HB formulated and syn‑ thesized foil‑backed nanofiber material; MAWG developed and executed antibacterial testing methodology, and oversaw on‑site testing. All authors contributed to manuscript preparation and review. All authors read and approved the final manuscript.
This work was supported in part by the Robert J. Reichlin High‑Performance Apparel Chair award to M. A. Sunderland.
Availability of data and materials
Raw data (image files and colony counts) generated for this study are archived on Labarchives.com, and available upon request from the corresponding author. Residual amounts of materials tested in this project are stored on‑site, and can be made using instructions provided in “Methods” section.
The authors declare that they have no competing interests.
1 Assistant Professor of Biology, Department of Biological and Chemical Sciences, College of Life Sciences, Thomas
Jefferson University, 4201 Henry Avenue, Philadelphia, PA 19144, USA. 2 Associate Professor of Engineering and Textiles,
Kanbar College of Design, Engineering, and Commerce, Thomas Jefferson University, 4201 Henry Avenue, Philadelphia, PA 19144, USA. 3 Professor and Program Director, Robert J. Reichlin High‑Performance Apparel Chair, Deputy Director
and Director of Engineering Technologies, Kanbar College of Design, Engineering, and Commerce, Thomas Jefferson University, 4201 Henry Avenue, Philadelphia, PA 19144, USA.
Received: 21 December 2018 Accepted: 6 May 2019
Appendino, G., Gibbons, S., Giana, A., Pagani, A., Grassi, G., Stavri, M., et al. (2008). Antibacterial cannabinoids from Cannabis sativa: A structure–activity study. Journal of Natural Products,71(8), 1427–1430.
Bhardwaj, N., & Kundu, S. C. (2010). Electrospinning: A fascinating fiber fabrication technique. Biotechnology Advances,28(3), 325–347. https ://doi.org/10.1016/j.biote chadv .2010.01.004.
Chouhan, S., Sharma, K., & Guleria, S. (2017). Antimicrobial activity of some essential oils—Present status and future perspec‑ tives. Medicines. https ://doi.org/10.3390/medic ines4 03005 8.
Dogan, H., Koral, M., & İnan, T. Y. (2009). Ag/Zn zeolite containing antibacterial coating for food‑packaging substrates. Journal of Plastic Film & Sheeting,25(3–4), 207–220. https ://doi.org/10.1177/87560 87909 35447 9.
Haase, H., Jordan, L., Keitel, L., Keil, C., & Mahltig, B. (2017). Comparison of methods for determining the effectiveness of anti‑ bacterial functionalized textiles. PLoS ONE. https ://doi.org/10.1371/journ al.pone.01883 04.
Latta, R. P., & Eaton, B. J. (1975). Seasonal fluctuations in cannabinoid content of Kansas Marijuana. Economic Botany,29(2), 153–163. https ://doi.org/10.1007/BF028 63315 .
Leizer, C., Ribnicky, D., Poulev, A., Dushenkov, S., & Raskin, I. (2000). The composition of hemp seed oil and its potential as an important source of nutrition. Journal of Nutraceuticals, Functional & Medical Foods,2(4), 35–53. https ://doi.org/10.1300/ J133v 02n04 _04.
Lelario, F., Scrano, L., De Franchi, S., Bonomo, M. G., Salzano, G., Milan, S., et al. (2018). Identification and antimicrobial activity of most representative secondary metabolites from different plant species. Chemical and Biological Technologies in Agricul-ture.. https ://doi.org/10.1186/s4053 8‑018‑0125‑0.
Neely, A. N., & Maley, M. P. (2000). Survival of enterococci and staphylococci on hospital fabrics and plastic. Journal of Clinical Microbiology,38(2), 724–726.
Schneider, C. A., Rasband, W. S., & Eliceiri, K. W. (2012). NIH image to ImageJ: 25 years of image analysis. Nature Methods,9(7), 671–675. https ://doi.org/10.1038/nmeth .2089.
Tachi, M., Hirabayashi, S., Yonehara, Y., Suzuki, Y., & Bowler, P. (2004). Development of an experimental model of infected skin ulcer. International Wound Journal,1(1), 49–55. https ://doi.org/10.1111/j.1742‑481x.2004.00006 .x.
Teufel, L., & Redl, B. (2006). Improved methods for the investigation of the interaction between textiles and microorganisms. Lenzinger Berichte,85, 54–60.